Abstract
The Ångströmsized probe of the scanning transmission electron microscope can visualize and collect spectra from single atoms. This can unambiguously resolve the chemical structure of materials, but not their isotopic composition. Here we differentiate between two isotopes of the same element by quantifying how likely the energetic imaging electrons are to eject atoms. First, we measure the displacement probability in graphene grown from either ^{12}C or ^{13}C and describe the process using a quantum mechanical model of lattice vibrations coupled with density functional theory simulations. We then test our spatial resolution in a mixed sample by ejecting individual atoms from nanoscale areas spanning an interface region that is far from atomically sharp, mapping the isotope concentration with a precision better than 20%. Although we use a scanning instrument, our method may be applicable to any atomic resolution transmission electron microscope and to other lowdimensional materials.
Introduction
Spectroscopy and microscopy are two fundamental pillars of materials science. By overcoming the diffraction limit of light, electron microscopy has emerged as a particularly powerful tool for studying lowdimensional materials such as graphene^{1}, in which each atom can be distinguished. Through advances in aberrationcorrected scanning transmission electron microscopy^{2,3} (STEM) and electron energy loss spectroscopy^{4,5}, the vision of a ‘synchrotron in a microscope’^{6} has now been realized. Spectroscopy of single atoms, including their spin state^{7}, has together with Zcontrast imaging^{3} allowed the identity and bonding of individual atoms to be unambiguously determined^{4,8,9,10}. However, discerning the isotopes of a particular element has not been possible—a technique that might be called ‘mass spectrometer in a microscope’.
Here we show how the quantum mechanical description of lattice vibrations lets us accurately model the stochastic ejection of single atoms^{11,12} from graphene consisting of either of the two stable carbon isotopes. Our technique rests on a crucial difference between electrons and photons when used as a microscopy probe: due to their finite mass, electrons can transfer significant amounts of momentum. When a highly energetic electron is scattered by the electrostatic potential of an atomic nucleus, a maximal amount of kinetic energy (inversely proportional to the mass of the nucleus, ∝) can be transferred when the electron backscatters. When this energy is comparable to the energy required to eject an atom from the material, defined as the displacement threshold energy T_{d}—for instance, when probing pristine^{11} or doped^{13} singlelayer graphene with 60–100 keV electrons—atomic vibrations become important in activating otherwise energetically prohibited processes due to the motion of the nucleus in the direction of the electron beam. The intrinsic capability of STEM for imaging further allows us to map the isotope concentration in selected nanoscale areas of a mixed sample, demonstrating the spatial resolution of our technique. The ability to do mass analysis in the transmission electron microscope thus expands the possibilities for studying materials on the atomic scale.
Results
Quantum description of vibrations
The velocities of atoms in a solid are distributed based on a temperaturedependent velocity distribution, defined by the vibrational modes of the material. Due to the geometry of a typical transmission electron microscopy (TEM) study of a twodimensional material, the outofplane velocity v_{z}, whose distribution is characterized by the mean square velocity , is here of particular interest. In an earlier study^{11} this was estimated using a Debye approximation for the outofplane phonon density of states^{14} (DOS) g_{z}(ω), where ω is the phonon frequency. A better justified estimate can be achieved by calculating the kinetic energy of the atoms via the thermodynamic internal energy, evaluated using the full phonon DOS.
As a starting point, we calculate the partition function Z=Tr{e^{−H/(kT)}}, where Tr denotes the trace operation and k is the Boltzmann constant and T the absolute temperature. We evaluate this trace for the secondquantized Hamiltonian H describing harmonic lattice vibrations^{15}:
where ħ is the reduced Planck constant, k the phonon wave vector, j the phonon branch index running to 3r (r being the number of atoms in the unit cell), ω_{j}(k) the eigenvalue of the j_{th} mode at k, and n_{j}(k) the number of phonons with frequency ω_{j}(k).
After computing the internal energy from the partition function via the Helmholtz free energy F=−kT lnZ, we obtain the Planck distribution function describing the occupation of the phonon bands (Methods). We must then explicitly separate the energy into the inplane U_{p} and outofplane U_{z} components, and take into account that half the thermal energy equals the kinetic energy of the atoms. This gives the outofplane mean square velocity of a single atom in a twoatom unit cell as
where M is the mass of the vibrating atom, ω_{z} is the highest outofplane mode frequency, and the correct normalization of the number of modes is included in the DOS.
Phonon dispersion
To estimate the phonon DOS, we calculated through density functional theory (DFT; GPAW package^{16,17}) the graphene phonon band structure^{18,19} via the dynamical matrix using the ‘frozen phonon method’ (Methods; Supplementary Fig. 1). Taking the density of the components corresponding to the outofplane acoustic (ZA) and optical (ZO) phonon modes (Supplementary Data 1) and solving equation 2 numerically, we obtain a mean square velocity m^{2}s^{−2} for a ^{12}C atom in normal graphene. This description can be extended to ‘heavy graphene’ (consisting of ^{13}C instead of a natural isotope mixture). A heavier atomic mass affects the velocity through two effects: the phonon band structure is scaled by the square root of the mass ratio (from the mass prefactor of the dynamical matrix), and the squared velocity is scaled by the mass ratio itself (equation 2). At room temperature, the first correction reduces the velocity by 3% in fully ^{13}C graphene compared with normal graphene, and the second one reduces it by an additional 10%, resulting in m^{2}s^{−2}.
Electron microscopy
In our experiments, we recorded time series at room temperature using the Nion UltraSTEM100 microscope, where each atom, or its loss, was visible in every frame. We chose small fields of view (∼1 × 1 nm^{2}) and short dwell times (8 μs) to avoid missing the refilling of vacancies (an example is shown in Fig. 1; likely this vacancy only appears to be unreconstructed due to the scanning probe). In addition to commercial monolayer graphene samples (Quantifoil R 2/4, Graphenea), we used samples of ^{13}C graphene synthesized by chemical vapour deposition (CVD) on Cu foils using ^{13}Csubstituted CH_{4} as carbon precursor, subsequently transferred onto Quantifoil TEM grids. An additional sample consisted of grains of ^{12}C and ^{13}C graphene on the same grid, synthesized by switching the precursor during growth (Methods).
From each experimental dataset (full STEM data available^{20}) within which a clear displacement was observed, we calculated the accumulated electron dose until the frame where the defect appeared (or a fraction of the frame if it appeared in the first one). The distribution of doses corresponds to a Poisson process^{12} whose expected value was found by loglikelihood minimization (Methods; Supplementary Fig. 2), directly yielding the probability of creating a vacancy (the dose data and statistical analyses are included in Supplementary Data 2). Figure 2 displays the corresponding displacement cross sections measured at voltages between 80 and 100 kV for normal (1.109% ^{13}C) and heavy graphene (∼99% ^{13}C), alongside values measured earlier^{11} using highresolution TEM (HRTEM). For lowprobability processes, the cross section is highly sensitive to both the atomic velocities and the displacement threshold energy. Since heavier atoms do not vibrate with as great a velocity, they receive less of a boost to the momentum transfer from an impinging electron. Thus, fewer ejections are observed for ^{13}C graphene.
Comparing theory with experiment
The theoretical total cross sections σ_{d}(T, E_{e}) are plotted in Fig. 2 for each voltage (Methods; Supplementary Table 1, Supplementary Data 2). The motion of the nuclei was included via a Gaussian distribution of atomic outofplane velocities P(v_{z}, T) characterized by the DFTcalculated , otherwise similar to the approach of ref. 11. A common displacement threshold energy was fitted to the data set by minimizing the varianceweighted mean square error (the 100 kV HRTEM point was omitted from the fitting, since it was underestimated probably due to the undetected refilling of vacancies, also seen in Fig. 1). The optimal T_{d} value was found to be 21.14 eV, resulting in a good description of all the measured cross sections. Notably, this is 0.8 eV lower than the earlier value calculated by DFT, and 2.29 eV lower than the earlier fit to HRTEM data^{11}. Different exchange correlation functionals we tested all overestimate the experimental value (by <1 eV), with the estimate T_{d}∈[21.25, 21.375] closest to experiment resulting from the C09 van der Waals functional^{21} (Methods).
Despite DFT overestimating the displacement threshold energy, we see from the good fit to the normal and heavy graphene data sets that our theory accurately describes the contribution of vibrations. Further, the HRTEM data and the STEM data are equally well described by the theory despite having several orders of magnitude different irradiation dose rates. This can be understood in terms of the very short lifetimes of electronic and phononic excitations in a metallic system^{22} compared with the average time between impacts. Even a very high dose rate of 10^{8} e^{−}Å^{−2}s^{−1} corresponds to a single electron passing through a 1 nm^{2} area every 10^{−10} s, whereas valence band holes are filled^{23} in <10^{−15} s and core holes^{24} in <10^{−14} s, while plasmons are damped^{25} within ∼10^{−13} s and phonons^{26} in ∼10^{−12} s. Our results thus show that multiple excitations do not contribute to the knockon damage in graphene, warranting another explanation (such as chemical etching^{11}) for the evidence linking a highly focused HRTEM beam to defect creation^{27}. Each impact is, effectively, an individual perturbation of the equilibrium state.
Local mapping of isotope concentration
Finally, to test the spatial resolution of our method, we studied a sample consisting of joined grains of ^{12}C and ^{13}C graphene. Isotope labelling combined with Raman spectroscopy mapping is a powerful tool for studying CVD growth of graphene^{28}, which is of considerable technological interest. Earlier studies have revealed the importance of carbon solubility into different catalyst substrates to control the growth process^{29}. However, the spatial resolution of Raman spectroscopy is limited, making it impossible to obtain atomicscale information of the transition region between grains of different isotopes.
The local isotope analysis is based on fitting the mean of the locally measured electron doses with a linear combination of doses generated by Poisson processes corresponding to ^{12}C and ^{13}C graphene using the theoretical cross section values. Although each dose results from a stochastic process, the expected doses for ^{12}C and ^{13}C are sufficiently different that measuring several displacements decreases the errors of their means well below the expected separation (Fig. 3c). To estimate the expected statistical variation for a certain number of measured doses, we generated a large number of sets of n Poisson doses, and calculated their means and standard errors as a function of the number of doses in each set. The calculated relative errors scale as 1/n and correspond to the precision of our measurement, which is better than 20% for as few as five measured doses in the ideal case. Although our accuracy is difficult to gauge precisely, by comparing the errors of the cross sections measured for isotopically pure samples to the fitted curve (Fig. 2), an estimate of roughly 5% can be inferred.
Working at 100 kV, we selected spots containing areas of clean graphene (43 in total) each only a few tens of nanometers in size (Fig. 1a), irradiating 4–15 (mean 7.8) fields of view 1 × 1 nm^{2} in size until the first displacement occurred (Fig. 1f). Comparing the mean of the measured doses to the generated data, we can estimate the isotope concentration responsible for such a dose. This assignment was corroborated by Raman mapping over the same area, allowing the two isotopes to be distinguished by their differing Raman shift. A general trend from ^{12}Crich to ^{13}Crich regions is captured by both methods (Fig. 3b), but a significant local variation in the measured doses is detectable (Fig. 3c). This variation indicates that the interfaces formed in a sequential CVD growth process may be far from atomically sharp^{30}, instead spanning a region of hundreds of nanometers, within which the carbon isotopes from the two precursors are mixed together.
Discussion
It is interesting to compare our method to established mass analysis techniques. In isotope ratio mass spectrometry precisions of 0.01% and accuracies of 1% have been reported^{31}. However, these measurements are not spatially resolved. For spatially resolved techniques, one of the most widely used is timeofflight secondary ion mass spectroscopy (ToFSIMS). It has a lateral resolution typically of several micrometers, which can be reduced to around 100 nm by finely focusing the ion beam^{32}. In the case of ToFSIMS, separation of the ^{13}C signal from ^{12}C^{1}H is problematic, resulting in a reported^{33} precision of 20% and an accuracy of ∼11%. The stateoftheart performance in local mass analysis can be achieved with atomprobe tomography^{34} (APT), which can record images with subnanometer spatial resolution in all three dimensions. A recent APT study of the ^{13}C/^{12}C ratio in detonation nanodiamonds reported a precision of 5%, but biases in the detection of differently charged ions limited accuracy to ∼25% compared to the natural isotope abundances^{35}.
A limitation of ToFSIMS is its inability to discriminate between the analyte and contaminants and that it requires uniform isotope concentrations over the beam area for accurate results. APT requires the preparation of specialized needlelike sample geometries, a laborious reconstruction process to analyse its results^{36}, and its detection efficiency is rather limited^{37}. In our case, we are only able to resolve relative mass differences between isotopes of the same element in the same chemical environment. While we do not need to resolve mass differences between different elements, since these differ in their scattering contrast, we do need to detect the ejection of single atoms, limiting the technique to atomically thin materials. However, our method captures the isotope information concurrently with atomic resolution imaging in a generalpurpose electron microscope, without the need for additional detectors.
We have shown how the Ångströmsized electron probe of a scanning transmission electron microscope can be used to estimate isotope concentrations via the displacement of single atoms. Although these results were achieved with graphene, our technique should work for any lowdimensional material, including hexagonal boron nitride and transition metal dichalcogenides such as MoS_{2}. This could potentially extend to van der Waals heterostructures^{38} of a few layers or other thin crystalline materials, provided a difference in the displacement probability of an atomic species can be uniquely determined. Neither is the technique limited to STEM: a parallel illumination TEM with atomic resolution would also work, although scanning has the advantage of not averaging the image contrast over the field of view. The areas we sampled were in total less than 340 nm^{2} in size, containing ∼6,600 carbon atoms of which 337 were ejected. Thus, while the nominal mass required for our complete analysis was already extremely small (131 zg), the displacement of only five atoms is required to distinguish a concentration difference of less than twenty per cent. Future developments in instrumentation may allow the massdependent energy transfer to be directly measured from highangle scattering^{39,40}, further enhancing the capabilities of STEM for isotope analysis.
Methods
Quantum model of vibrations
The outofplane mean square velocity can be estimated by calculating the kinetic energy via the thermodynamic internal energy using the outofplane phonon DOS g_{z}(ω), where ω is the phonon frequency. In the second quantization formalism, the Hamiltonian for harmonic lattice vibrations is ref. 15
where k is the phonon wave vector, j is the phonon branch index running to 3r (r being the number of atoms in the unit cell), ω_{j}(k) the eigenvalue of the j_{th} mode at k, and and b_{k j} are the phonon creation and annihilation operators, respectively.
Using the partition function Z=Tr{e^{−H/(kT)}}, where Tr denotes the trace operation and k is the Boltzmann constant and T the absolute temperature, and evaluating the trace using this Hamiltonian, we have
where is the number of phonons with frequency ω_{j}(k).
The Helmholtz free energy is thus
and the internal energy of a single unit cell, therefore, becomes^{15}
where in the last step the sum is expressed as an average over the phonon DOS. Using the identity yields the Planck distribution function describing the occupation of the phonon bands, and explicitly dividing the energy into the inplane U_{p} and outofplane U_{z} components, we can rewrite this as
where the number of modes is included in the normalization of the DOSes, that is, , corresponding to the outofplane acoustic (ZA) and optical (ZO) modes (the inplane DOS g_{p}(ω) being correspondingly normalized to 4), and ω_{d} is the highest frequency of the highest phonon mode.
Since half of the thermal energy equals the average kinetic energy of the atoms, and the graphene unit cell has two atoms, the outofplane kinetic energy of a single atom is
Thus, the outofplane mean square velocity of an atom becomes
where ω_{z} is now the highest outofplane mode frequency. This can be solved numerically for a known g_{z}(ω).
For the inplane vibrations, we would equivalently get
Frozen phonon calculation
To estimate the phonon DOS, we calculated the graphene phonon band structure via the dynamical matrix, which was computed by displacing each of the two primitive cell atoms by a small displacement (0.06 Å) and calculating the forces on all other atoms in a 7 × 7 supercell (‘frozen phonon method’; the cell size is large enough so that the forces on the atoms at its edges are negligible) using DFT as implemented in the gridbased projectoraugmented wave code (GPAW) package^{17}. Exchange and correlation were described by the local density approximation^{41}, and a Γcentered MonkhorstPack kpoint mesh of 42 × 42 × 1 was used to sample the Brillouin zone. A fine computational grid spacing of 0.14 Å was used alongside strict convergence criteria for the structural relaxation (forces <10^{−5} eVÅ^{−1} per atom) and the selfconsistency cycle (change in eigenstates <10^{−13} eV^{2} per electron). The resulting phonon dispersion (Supplementary Fig. 1) describes well the quadratic dispersion of the ZA mode near Γ, and is in excellent agreement with earlier studies^{18,19}. Supplementary Data 1 contains the outofplane phonon DOS.
Graphene synthesis and transfer
In addition to commercial monolayer graphene (Graphenea QUANTIFOIL R 2/4), our graphene samples were synthesized by CVD in a furnace equipped with two separate gas inlets that allow for independent control over the two isotope precursors^{29} (that is, either ∼99% ^{12}CH_{4} or ∼99% ^{13}CH_{4} methane). The asreceived 25 μm thick 99.999% pure Cu foil was annealed for ∼1 h at 960 °C in a 1:20 hydrogen/argon mixture with a pressure of ∼10 mbar. The growth of graphene was achieved by flowing 50 cm^{3} min^{−1} of CH_{4} over the annealed substrate while keeping the Ar/H_{2} flow, temperature and pressure constant. For the isotopically mixed sample with separated domains, the annealing and growth temperature was increased to 1,045 °C and the flow rate decreased to 2 cm^{3} min^{−1}. After introducing ^{12}CH_{4} for 2 min the carbon precursor flow was stopped for 10 s, and the other isotope precursor subsequently introduced into the chamber for another 2 min. This procedure was repeated with a flow time of 1 min. After the growth, the CH_{4} flow was interrupted and the heating turned off, while the Ar/H_{2} flow was kept unchanged until the substrate reached room temperature. The graphene was subsequently transferred onto a holey amorphous carbon film supported by a TEM grid using a direct transfer method without using polymer^{42}.
Scanning transmission electron microscopy
Electron microscopy experiments were conducted using a Nion UltraSTEM100 scanning transmission electron microscope, operated between 80 and 100 kV in nearultrahigh vacuum (2 × 10^{−7} Pa). The instrument was aligned for each voltage so that atomic resolution was achieved in all of the experiments. The beam current during the experiments varied between 8 and 80 pA depending on the voltage, corresponding to dose rates of ∼5–50 × 10^{7} e^{−}Å^{−2}s^{−1}. The beam convergence semiangle was 30 mrad and the semiangular range of the mediumangle annulardarkfield detector was 60–200 mrad.
Poisson analysis
Assuming the displacement data are stochastic, the waiting times (or, equivalently, the doses) should arise from a Poisson process with mean λ. Thus the probability to find k events in a given time interval follows the Poisson distribution
To estimate the Poisson expectation value for each sample and voltage, the cumulative doses of each data set were divided into bins of width w (using onelevel recursive approximate Wand binning^{43}), and the number of bins with 0, 1, 2... occurrences were counted. The goodness of the fits was estimated by calculating the Cash Cstatistic^{44} (in the asymptoticallyχ^{2} formulation^{45}) between a fitted Poisson distribution and the data:
where N is the number of occurence bins, n_{i} is the number of events in bin i, and e_{i} is the expected number of events in bin i from a Poisson process with mean λ.
An error estimate for the mean was calculated using the approximate confidence interval proposed for Poisson processes with small means and small sample sizes by Khamkong^{46}:
where is the estimated mean and Z_{2.5} is the normal distribution single tail cumulative probability corresponding to a confidence level of (100−α)=95%, equal to 1.96.
The statistical analyses were conducted using the Wolfram Mathematica software (version 10.5), and the Mathematica notebook is included as Supplementary Data 2. Outputs of the Poisson analyses for the main data sets of normal and heavy graphene as a function of voltage are additionally shown as Supplementary Fig. 2.
Displacement cross section
The energy transferred to an atomic nucleus from a fast electron as a function of the electron scattering angle θ is ref. 47
which is valid also for a moving target nucleus for electron energies >10 keV as noted by Meyer and coworkers^{11}. For purely elastic collisions (where the total kinetic energy is conserved), the maximum transferred energy E_{max} corresponds to electron backscattering, that is, θ=π. However, when the impacted atom is moving, E_{max} will also depend on its speed.
To calculate the cross section, we use the approximation of McKinley and Feshbach^{48} of the original series solution of Mott to the Dirac equation, which is very accurate for lowZ elements and subMeV beams. This gives the cross section as a function of the electron scattering angle as
where β=v/c is the ratio of electron speed to the speed of light (0.446225 for 60 keV electrons) and σ_{R} is the classical Rutherford scattering cross section
Using equation 14 this can be rewritten as a function of the transferred energy^{49} as
Distribution of atomic vibrations
The maximum energy (in eV) that an electron with mass m_{e} and energy E_{e}=eU (corresponding to acceleration voltage U) can transfer to a nucleus of mass M that is moving with velocity v is
where and are the relativistic energies of the electron and the nucleus, and E_{n}=Mv^{2}/2 the initial kinetic energy of the nucleus in the direction of the electron beam.
The probability distribution of velocities of the target atoms in the direction parallel to the electron beam follows the normal distribution with a standard deviation equal to the temperaturedependent mean square velocity ,
Total cross section with vibrations
The cross section is calculated by numerically integrating equation 17 multiplied by the Gaussian velocity distribution (equation 19) over all velocities v where the maximum transferred energy (equation 18) exceeds the displacement threshold energy T_{d}:
where E_{max}(v, E_{e}) is given by equation 18, the term Θ[E_{max}(v, E_{e})−E_{d}] is the Heaviside step function, T is the temperature and E_{e} is the electron kinetic energy. The upper limit for the numerical integration v_{max}=8 was chosen so that the velocity distribution is fully sampled.
Displacement threshold simulation
For estimating the displacement threshold energy, we used DFT molecular dynamics as established in our previous studies^{12,13,50,51}. The threshold was obtained by increasing the initial kinetic energy of a target atom until it escaped the structure during the molecular dynamics run. The calculations were performed using the gridbased projectoraugmented wave code (GPAW), with the computational grid spacing set to 0.18 Å. The molecular dynamics calculations employed a double zeta linear combination of atomic orbitals basis^{52} for a 8 × 6 unit cell of 96 atoms, with a 5 × 5 × 1 MonkhorstPack kpoint grid^{53} used to sample the Brillouin zone. A timestep of 0.1 fs was used for the VelocityVerlet dynamics^{54}, and the velocities of the atoms initialized by a Maxwell–Boltzmann distribution at 50 K, equilibrated for 20 timesteps before the simulated impact.
To describe exchange and correlation, we used the local density approximation^{41}, and the PerdewBurkeErnzerhof (PBE)^{55}, PerdewWang 1991 (PW91, ref. 41), RPBE^{56} and revPBE^{57} functionals, yielding displacement threshold energies of 23.13, 21.88, 21.87, 21.63 and 21.44 eV (these values are the means of the highest simulated kinetic energies that did not lead to an ejection and the lowest that did, respectively). Additionally, we tested the C09 (ref. 21) functional to see whether inclusion of the van der Waals interaction would affect the results. This does bring the calculated threshold energy down to [21.25, 21.375] eV, in better agreement with the experimental fit. However, a more precise algorithm for the numerical integration of the equations of motion, more advanced theoretical models for the interaction, or timedependent DFT may be required to improve the accuracy of the simulations further.
Varying mean square velocity with concentration
Since the phonon dispersion of isotopically mixed graphene gives a slightly different outofplane mean square velocity for the atomic vibrations, for calculating the cross section for each concentration, we assumed the velocity of mixed concentration areas to be linearly proportional to the concentration
where c is the concentration of ^{12}C and v_{12/13} are the atomic velocities for normal and heavy graphene, respectively.
Raman spectroscopy
A Raman spectrometer (NT MDT Ntegra Spectra) equipped with a 532 nm excitation laser was used for Raman measurements. A computercontrolled stage allowed recording a Raman spectrum map over the precise hole on which the electron microscopy measurements were conducted, which was clearly identifiable from neighboring spot contamination and broken film holes.
The frequencies ω of the optical phonon modes vary with the atomic mass M as ω∝M^{−1/2} due to the mass prefactor of the dynamical matrix. This makes the Raman shifts of ^{13}C graphene (12/13)^{−1/2} times smaller, allowing the mapping and localization of ^{12}C and ^{13}C domains^{28} with a spatial resolution limited by the size of the laser spot (nominally ∼400 nm). The shifts of the G and 2D bands compared with a corresponding normal graphene sample are given by , where ω_{12} is the G (2D) line frequency of the normal sample, c_{0}^{13}=0.01109 is the natural abundance of ^{13}C, and c is the unknown concentration of ^{12}C in the measured spot.
Due to background signal arising from the carbon support film of the TEM grid, we analyzed the shift of the 2D band, where two peaks were in most locations present in the spectrum. However, in many spectra these did not correspond to either fully ^{12}C or ^{13}C graphene^{58}, indicating isotope mixing within the Raman coherence length. To assign a single value to the ^{12}C concentration for the overlay of Fig. 3, we took into account both the shifts of the peaks (to estimate the nominal concentration for each signal) and their areas (to estimate their relative abundances) as follows:
where are the nominal concentrations of ^{12}C determined from the measured higher and lower 2D Raman shift peak positions, ω_{A/B} are the measured peak centers of the higher and lower 2D signals, and A and B are their integrated intensities. The peak positions of fully ^{12}C and ^{13}C graphene were taken from the highest and lowest peak positions in the entire mapped area (covering several dozen Quantifoil holes), giving ω_{12}=2,690 cm^{−1} and ω_{13}=2,600 cm^{−1}. The fitted 2D spectra, arranged in the same 6 × 6 grid as the overlay, can be found as Supplementary Fig. 3
Data availability
The full STEM time series data on which the determination of the ^{12}C and ^{13}C displacement cross sections (Fig. 2) are based are available on figshare with the identifier http://dx.doi.org/10.6084/m9.figshare.c.3311946 (ref. 20). The STEM data of Fig. 3 are available upon request. All other data are contained within the article and its Supplementary Information files.
Additional information
How to cite this article: Susi, T. et al. Isotope analysis in the transmission electron microscope. Nat. Commun. 7, 13040 doi: 10.1038/ncomms13040 (2016).
Change history
30 August 2017
A correction has been published and is appended to both the HTML and PDF versions of this paper. The error has not been fixed in the paper.
References
Geim, A. K. & Novoselov, K. S. The rise of graphene. Nat. Mater. 6, 183–191 (2007).
Nellist, P. D. et al. Direct subAngstrom imaging of a crystal lattice. Science 305, 1741 (2004).
Krivanek, O. L. et al. Atombyatom structural and chemical analysis by annular darkfield electron microscopy. Nature 464, 571–574 (2010).
Suenaga, K. & Koshino, M. Atombyatom spectroscopy at graphene edge. Nature 468, 1088–1090 (2010).
Krivanek, O. L. et al. Vibrational spectroscopy in the electron microscope. Nature 514, 209–212 (2014).
Brown, L. M. Proceedings of the institute of physics electron microscopy and analysis group conference, Cavendish Laboratory, University of Cambridge, 2–5 September 1997. In Rodenburg J. M. (ed.) Electron Microscopy and Analysis 1997., Vol. 191 of Conference Series Number 153 17–22 Institute of Physics Publishing Blackwell Science Ltd (1998).
Lin, Y.C., Teng, P.Y., Chiu, P.W. & Suenaga, K. Exploring the single atom spin state by electron spectroscopy. Phys. Rev. Lett. 115, 206803 (2015).
Zhou, W. et al. Direct determination of the chemical bonding of individual impurities in graphene. Phys. Rev. Lett. 109, 206803 (2012).
Ramasse, Q. M. et al. Probing the bonding and electronic structure of single atom dopants in graphene with electron energy loss spectroscopy. Nano Lett. 13, 4989–4995 (2013).
Kepaptsoglou, D. et al. Electronic structure modification of ion implanted graphene: the spectroscopic signatures of p and ntype doping. ACS Nano 9, 11398–11407 (2015).
Meyer, J. C. et al. Accurate measurement of electron beam induced displacement cross sections for singlelayer graphene. Phys. Rev. Lett. 108, 196102 (2012).
Susi, T. et al. Siliconcarbon bond inversions driven by 60keV electrons in graphene. Phys. Rev. Lett. 113, 115501 (2014).
Susi, T. et al. Atomistic description of electron beam damage in nitrogendoped graphene and singlewalled carbon nanotubes. ACS Nano 6, 8837–8846 (2012).
Tewary, V. K. & Yang, B. Singular behavior of the DebyeWaller factor of graphene. Phys. Rev. B 79, 125416 (2009).
Böttger, H. Principles of the Theory of Lattice Dynamics PhysicaVerlag Weinheim (1983).
Mortensen, J., Hansen, L. & Jacobsen, K. Realspace grid implementation of the projector augmented wave method. Phys. Rev. B 71, 035109 (2005).
Enkovaara, J. et al. Electronic structure calculations with GPAW: a realspace implementation of the projector augmentedwave method. J. Phys. Condens. Matter 22, 253202 (2010).
Wirtz, L. & Rubio, A. The phonon dispersion of graphite revisited. Solid State Commun. 131, 141–152 (2004).
Mohr, M. et al. Phonon dispersion of graphite by inelastic xray scattering. Phys. Rev. B 76, 035439 (2007).
Susi, T. et al. Atomic resolution electron irradiation time series of isotopically labeled monolayer graphene. figsharehttp://dx.doi.org/10.6084/m9.figshare.c.3311946 (2016).
Cooper, V. R. Van der waals density functional: an appropriate exchange functional. Phys. Rev. B 81, 161104 (2010).
Egerton, R., McLeod, R., Wang, F. & Malac, M. Basic questions related to electroninduced sputtering in the TEM. Ultramicroscopy 110, 991–997 (2010).
Egerton, R. Control of radiation damage in the TEM. Ultramicroscopy 127, 100–108 (2013).
Brühwiler, P. A. et al. π* and σ* excitons in C 1s absorption of graphite. Phys. Rev. Lett. 74, 614–617 (1995).
Yan, H. et al. Damping pathways of midinfrared plasmons in graphene nanostructures. Nat. Photon. 7, 394–399 (2013).
Kang, K., Abdula, D., Cahill, D. G. & Shim, M. Lifetimes of optical phonons in graphene and graphite by timeresolved incoherent antiStokes Raman scattering. Phys. Rev. B 81, 165405 (2010).
Robertson, A. W. et al. Spatial control of defect creation in graphene at the nanoscale. Nat. Commun. 3, 1144 (2012).
Frank, O., Kavan, L. & Kalbac, M. Carbon isotope labelling in graphene research. Nanoscale 6, 6363–6370 (2014).
Li, X., Cai, W., Colombo, L. & Ruoff, R. S. Evolution of graphene growth on Ni and Cu by carbon isotope labeling. Nano Lett. 9, 4268–4272 (2009).
Liu, L. et al. Heteroepitaxial growth of twodimensional hexagonal boron nitride templated by graphene edges. Science 343, 163–167 (2014).
Muccio, Z. & Jackson, G. P. Isotope ratio mass spectrometry. Analyst 134, 213–222 (2009).
Benninghoven, A. Chemical analysis of inorganic and organic surfaces and thin films by static timeofflight secondary ion mass spectrometry (TOFSIMS). Angew. Chem. Int. Ed. (English) 33, 1023–1043 (1994).
Stephan, T. TOFSIMS in cosmochemistry. Planet. Space Sci. 49, 859–906 (2001).
Gault, B., Moody, M. P., Cairney, J. M. & Ringer, S. P. Atom Probe Microscopy Vol. 160, Springer Science & Business Media (2012).
Lewis, J. B., Isheim, D., Floss, C. & Seidman, D. N. ^{12}C/^{12}Cratio determination in nanodiamonds by atomprobe tomography. Ultramicroscopy 159, 248–254 (2015).
Baik, S.I. et al. An atomistic tomographic study of oxygen and hydrogen atoms and their molecules in CVD grown graphene. Small 11, 5968–5974 (2015).
Kelly, T. F. & Miller, M. K. Atom probe tomography. Rev. Sci. Instrum. 78, 031101 (2007).
Geim, A. K. & Grigorieva, I. V. Van der Waals heterostructures. Nature 499, 419–425 (2013).
Lovejoy, T. et al. Energyfiltered highangle dark field mapping of ultralight elements. Microsc. Microanal. 20, 558–559 (2014).
Argentero, G., Mangler, C., Kotakoski, J., Eder, F. & Meyer, J. Towards weighing individual atoms by highangle scattering of electrons. Ultramicroscopy 151, 23–30 (2015).
Perdew, J. P. & Wang, Y. Accurate and simple analytic representation of the electrongas correlation energy. Phys. Rev. B 45, 13244–13249 (1992).
Regan, W. et al. A direct transfer of layerarea graphene. Appl. Phys. Lett. 96, 113102 (2010).
Wand, M. P. Databased choice of histogram bin width. Am. Statistician 51, 59–64 (1997).
Cash, W. Parameter estimation in astronomy through application of the likelihood ratio. Astrophys. J. 228, 939–947 (1979).
Aschwanden, M. J. & Schmahl, E. RHESSI Team. Reconstruction of RHESSI solar flare images with a forward fitting method. In Lin R. P., Dennis B. R., Benz A. O. (eds) The Reuven Ramaty HighEnergy Solar Spectroscopic Imager (RHESSI) 193–211Springer (2003).
Khamkong, M. Approximate confidence interval for the mean of poisson distribution. Open J. Stat. 02, 204–207 (2012).
Mott, N. F. & Massey, H. The Theory of Atomic Collisions 3rd edn Clarendon Press (1965).
McKinley, W. A. Jr & Feshbach, H. The Coulomb scattering of relativistic electrons by nuclei. Phys. Rev. 74, 1759–1763 (1948).
Zobelli, A., Gloter, A., Ewels, C. P., Seifert, G. & Colliex, C. Electron knockon cross section of carbon and boron nitride nanotubes. Phys. Rev. B 75, 245402 (2007).
Kotakoski, J. et al. Stonewalestype transformations in carbon nanostructures driven by electron irradiation. Phys. Rev. B 83, 245420 (2011).
Kotakoski, J., SantosCottin, D. & Krasheninnikov, A. V. Stability of graphene edges under electron beam: equilibrium energetics versus dynamic effects. ACS Nano 6, 671–676 (2012).
Larsen, A. H., Vanin, M., Mortensen, J. J., Thygesen, K. S. & Jacobsen, K. W. Localized atomic basis set in the projector augmented wave method. Phys. Rev. B 80, 195112 (2009).
Monkhorst, H. J. & Pack, J. D. Special points for Brillouinzone integrations. Phys. Rev. B 13, 5188–5192 (1976).
Swope, W. C., Andersen, H. C., Berens, P. H. & Wilson, K. R. A computer simulation method for the calculation of equilibrium constants for the formation of physical clusters of molecules: application to small water clusters. J. Chem. Phys. 76, 637–649 (1982).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).
Hammer, B., Hansen, L. & Nørskov, J. Improved adsorption energetics within densityfunctional theory using revised PerdewBurkeErnzerhof functionals. Phys. Rev. B 59, 7413 (1999).
Zhang, Y. & Yang, W. Comment on ‘Generalized gradient approximation made simple’. Phys. Rev. Lett. 80, 890–890 (1998).
Carvalho, B. R. et al. Probing carbon isotope effects on the raman spectra of graphene with different ^{13}C concentrations. Phys. Rev. B 92, 125406 (2015).
Acknowledgements
T.S. acknowledges funding from the Austrian Science Fund (FWF) via project P 28322N36, and the computational resources of the Vienna Scientific Cluster. J.K. acknowledges funding from the Wiener Wissenschafts, Forschungs und Technologiefonds (WWTF) via project MA14009. C.H., G.A., C.M. and J.C.M. acknowledge funding by the European Research Council Grant No. 336453PICOMAT. T.J.P. was supported by the European Union’s Horizon 2020 research and innovation programme under the Marie SkłodowskaCurie grant agreement No. 655760DIGIPHASE. We further thank Ondrej Krivanek for useful feedback.
Author information
Authors and Affiliations
Contributions
T.S. performed theoretical and statistical analyses and DFT simulations, participated in STEM experiments and their analysis, and drafted the manuscript. C.H. performed sample synthesis, and participated in STEM experiments, their analysis, and the Raman analysis. G.A. participated in sample synthesis and the Raman analysis. G.T.L. participated in STEM experiments and their analysis. C.M. and T.J.P. prepared special alignments for the STEM instrument with J.K., who supervised the theoretical and statistical analyses and STEM experiments. J.K. and J.C.M conceived and supervised the study.
Corresponding authors
Ethics declarations
Competing interests
T.S., J.C.M. and J.K. are named on a patent application relating to this method of isotope analysis (application number EP16183371). All other authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 13 and Supplementary Table 1 (PDF 2297 kb)
Supplementary Data 1
The outofplane components of the graphene phonon density of states. (TXT 195 kb)
Supplementary Data 2
A Wolfram Mathematica (version 10.5) notebook containing the dose data and its statistical analyses. (TXT 940 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Susi, T., Hofer, C., Argentero, G. et al. Isotope analysis in the transmission electron microscope. Nat Commun 7, 13040 (2016). https://doi.org/10.1038/ncomms13040
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms13040
This article is cited by

Imaging of isotope diffusion using atomicscale vibrational spectroscopy
Nature (2022)

Towards chirality control of graphene nanoribbons embedded in hexagonal boron nitride
Nature Materials (2021)

Quantifying transmission electron microscopy irradiation effects using twodimensional materials
Nature Reviews Physics (2019)

Influence of temperature on the displacement threshold energy in graphene
Scientific Reports (2019)

In situ control of graphene ripples and strain in the electron microscope
npj 2D Materials and Applications (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.